# HEXAGONAL CRYSTALS

In document Fundamentals of Materials Science and Engineering 5th Edition pdf (Page 73-77)

A problem arises for crystals having hexagonal symmetry in that some crystallo- graphic equivalent directions will not have the same set of indices. This is circum- vented by utilizing a four-axis, or Miller–Bravais, coordinate system as shown in

Figure 3.21. The three a1, a2, and a3axes are all contained within a single plane z + y y O a a a [110] Direction P x a a a1 a2 a3 z 120°

FIGURE3.21 Coordinate axis system for a hexagonal unit cell

(called the basal plane), and at 120⬚angles to one another. The z axis is perpendicular to this basal plane. Directional indices, which are obtained as described above, will be denoted by four indices, as [uvtw]; by convention, the first three indices pertain

to projections along the respective a1, a2, and a3axes in the basal plane.

Conversion from the three-index system to the four-index system, [uvw⬘] —씮[uvtw]

is accomplished by the following formulas:

un 3(2u⬘ ⫺v⬘) (3.7a) vn 3(2v⬘ ⫺u⬘) (3.7b) t⫽ ⫺(uv) (3.7c) wnw⬘ (3.7d)

where primed indices are associated with the three-index scheme and unprimed, with the new Miller–Bravais four-index system; n is a factor that may be required to reduce u,v, t, and w to the smallest integers. For example, using this conversion, the [010] direction becomes [1210]. Several different directions are indicated in the hexagonal unit cell (Figure 3.22a).

RYSTALLOGRAPHIC

### P

LANES

The orientations of planes for a crystal structure are represented in a similar manner. Again, the unit cell is the basis, with the three-axis coordinate system as represented in Figure 3.19. In all but the hexagonal crystal system, crystallographic planes are specified by three Miller indices as (hkl). Any two planes parallel to each other are equivalent and have identical indices. The procedure employed in determination of the h, k, and l index numbers is as follows:

1. If the plane passes through the selected origin, either another parallel

plane must be constructed within the unit cell by an appropriate transla- tion, or a new origin must be established at the corner of another unit cell.

2. At this point the crystallographic plane either intersects or parallels each

of the three axes; the length of the planar intercept for each axis is determined in terms of the lattice parameters a, b, and c.

54Chapter 3 / Structures of Metals and Ceramics

[0001] (0001) [1120]` [1100]` (1010) (1011)` a1 a1 a2 a3 a3 z z (a) (b) `

FIGURE3.22 For the

hexagonal crystal system, (a) [0001], [1100], and [1120] directions, and (b) the (0001), (1011), and (1010) planes.

3.13 Crystallographic Planes55 z x y z x y z x y (b) (c) (a) O (001) Plane referenced to the origin at point O

(111) Plane referenced to the origin at point O

(110) Plane referenced to the origin at point O Other equivalent (001) planes Other equivalent (111) planes Other equivalent (110) planes O O FIGURE3.23 Representations of a series each of (a) (001), (b) (110), and (c) (111) crystallographic planes.

3. The reciprocals of these numbers are taken. A plane that parallels an

axis may be considered to have an infinite intercept, and, therefore, a zero index.

4. If necessary, these three numbers are changed to the set of smallest

integers by multiplication or division by a common factor.2

5. Finally, the integer indices, not separated by commas, are enclosed within

parentheses, thus: (hkl).

An intercept on the negative side of the origin is indicated by a bar or minus sign positioned over the appropriate index. Furthermore, reversing the directions of all indices specifies another plane parallel to, on the opposite side of and equidis- tant from, the origin. Several low-index planes are represented in Figure 3.23.

One interesting and unique characteristic of cubic crystals is that planes and directions having the same indices are perpendicular to one another; however, for other crystal systems there are no simple geometrical relationships between planes and directions having the same indices.

2On occasion, index reduction is not carried out(e.g., for x-ray diffraction studies that are

described in Section 3.19);其for example, (002) is not reduced to (001). In addition, for ceramic materials, the ionic arrangement for a reduced-index plane may be different from that for a nonreduced one.

56Chapter 3 / Structures of Metals and Ceramics z y x a b O c z y x (a) (b) x b c/2 (012) Plane z O O ⬘ ⬘ ⬘

XAMPLE

ROBLEM

### 3.9

Determine the Miller indices for the plane shown in the accompanying sketch (a).

### S

O L U T I O N

Since the plane passes through the selected origin O, a new origin must be chosen at the corner of an adjacent unit cell, taken as O⬘and shown in sketch (b). This plane is parallel to the x axis, and the intercept may be taken asa.

The y and z axes intersections, referenced to the new origin O⬘, are ⫺b and c/2, respectively. Thus, in terms of the lattice parameters a, b, and c, these

intersections are앝,⫺1, and. The reciprocals of these numbers are 0,⫺1, and 2; and since all are integers, no further reduction is necessary. Finally, enclosure in parentheses yields (012).

These steps are briefly summarized below:

x y z

Intercepts 앝ab c/2

Intercepts (in terms of lattice parameters) 앝 ⫺1 Reciprocals 0 ⫺1 2 Reductions (unnecessary)

Enclosure (012)

XAMPLE

ROBLEM

### 3.10

Construct a (011) plane within a cubic unit cell.

### S

O L U T I O N

To solve this problem, carry out the procedure used in the preceding example in reverse order. To begin, the indices are removed from the parentheses, and reciprocals are taken, which yields앝,⫺1, and 1. This means that the particular plane parallels the x axis while intersecting the y and z axes atb and c,

respectively, as indicated in the accompanying sketch (a). This plane has been drawn in sketch (b). A plane is indicated by lines representing its intersections with the planes that constitute the faces of the unit cell or their extensions. For example, in this figure, line ef is the intersection between the (011) plane and

3.13 Crystallographic Planes57

the top face of the unit cell; also, line gh represents the intersection between this same (011) plane and the plane of the bottom unit cell face extended. Similarly, lines eg and fh are the intersections between (011) and back and front cell faces, respectively.

In document Fundamentals of Materials Science and Engineering 5th Edition pdf (Page 73-77)